Pages

Tuesday, 26 May 2009

Manufacturing Process of Nylon 6,6

Manufacturing Process of Nylon 6,6

Nylon 6,6 is made from Hexamethylene diamine and adipic acid as shown in the figure below.

Spinning of Nylon 6,6

The chips of nylon polymer are fed through a hopper A, into a spinning vessel B, on an electrically heated grid ( perforated plate) C. The perforations are so small that the chips do not pass through, but when melted, the liquid can pass.

The molten nylon collects as a pool D, at the bottom of the vessel. This liquid should not come into contact with oxygen or air and hence nitrogen is introduced into the vessel. The molten polymer is kept at a temperature of about 288 deg C and sucked by a pump F, into a spinnerette E. The molten polymer solidifies as soon as it emerges out of the spinnerette. The filament thus formed pass through a colloing zone, in which cold air G circulates directed towards the filaments. The filaments are then passed through a steam chamber H, to wet them before winding on the bobbin L.

Drawing

Nylon filaments as obtained are not very strong. They have to tbe drawn 4-7 times their original length. This is done by cold drawing. The yarn in pulled off from bobbin L through guides M and N, between a pair of rollers O. The speed of rotation of these rollers determines the initial speed. The yarn then goes over a deflector P, and two to three times around roller Q, running at five times the speed than that of O. The yarn subsequently courses through another guide R, and wound on another bobbin which rotates at very high speed, to impart twist in the yarn before being wound.